Expression, Cross-Linking, and Characterization of ... ? Expression, Cross-Linking, and Characterization
Post on 07-Sep-2018
Expression, Cross-Linking, and Characterization ofRecombinant Chitin Binding Resilin
Guokui Qin,, Shaul Lapidot,, Keiji Numata, Xiao Hu,,| Sigal Meirovitch, Mara Dekel,
Itai Podoler, Oded Shoseyov,*, and David L. Kaplan*,
Department of Biomedical Engineering, 4 Colby Street, Tufts University, Medford, Massachusetts 02155,Department of Physics and Astronomy, Tufts University, Medford, Massachusetts 02155, and The RobertH. Smith Institute of Plant Sciences and Genetics in Agriculture, Robert H. Smith Faculty of Agriculture,
Food and Environment, The Hebrew University of Jerusalem, P.O. Box 12, Rehovot 76100, Israel
Received June 30, 2009; Revised Manuscript Received September 9, 2009
Resilin is a polymeric rubber-like protein secreted by insects to specialized cuticle regions, in areas where highresilience and low stiffness are required. Resilin binds to the cuticle polysaccharide chitin via a chitin bindingdomain and is further polymerized through oxidation of the tyrosine residues resulting in the formation of dityrosinebridges and assembly of a high-performance protein-carbohydrate composite material. We describe the mechanical,structural and biochemical function of chitin binding recombinant Drosophila melanogaster resilin. Various resilinconstructs were cloned including the full length gene enabling Ni-NTA purification, as well as heat and saltprecipitation for rapid and efficient purification. The binding isotherms and constants (Kd, Bmax) of resilin tochitin via its chitin binding domain were determined and displayed high affinity to chitin, implying its importantrole in the assembly of the resilin-chitin composite. The structural and elastic properties were investigated usingFourier transform infrared spectroscopy, circular dichroism, and atomic force microscopy with peroxidase cross-linked solid resilin materials. Generally, little structural organization was found by these biophysical methods,suggesting structural order was not induced by the dityrosine cross-links. Further, the elastomeric properties foundfrom the full length protein compared favorably with the shorter resilin generated previously from exon 1. Theunusual elastomeric behavior of this protein suggests possible utility in biomaterials applications.
IntroductionResilin was discovered in 1960 in studies on the flight
mechanisms of desert locusts (Schistocerca gregaria) anddragonflies (Aeshna juncea).1 The protein is found withinstructures where energy storage and long-range elasticity areneeded, such as the flight system of locusts,1 the jumpingmechanism of fleas,2 and the sound producing organ of cicadas.3
Resilin behaves like an entropic elastomer,1 and was initiallyproposed to consist of randomly coiled protein chains linkedby stable covalent cross-links, the elastic force being accountedfor by a decrease in conformational entropy when the materialwas strained.4,5 Furthermore, it was reported that resilin couldbe stretched up to 3-4 times its original length before breaking,and immediately snap back to its resting length upon release ofthe tensile force showing no deformation.6 Resilin is insolublein media which does not degrade peptide bonds and is stableup to 140 C.5 Further, resilin possesses high resilience, 92%or more, and a very high fatigue lifetime,7,8 due to the covalentcross-linkage between tyrosine residues, generating di- andtrityrosines.9
Earlier studies of resilin including electron microscopy andX-ray diffraction suggested that resilin is an unstructuredamorphous protein matrix.8,10 Recent studies have providedcompelling evidence that the crossslinking of resilin in insects
is mediated through the action of peroxidases.8,11 To date,structural studies of resilin are limited. A structural descriptionof the synthetic construct resilin AN16 was completed bynuclear magnetic resonance spectroscopy (NMR) and Ramanand it was suggested that the resilin chains are mobile.12
Ardell and Andersen identified the Drosophila melanogasterresilin gene and reported two significant elastic repeat motifs;an N-terminal domain comprising 18 pentadecapeptide repeats(GGRPSDSYGAPGGGN) and a C-terminal domain comprising11 tridecapeptide repeats (GYSGGRPGGQDLG).13 Each repeatis found entirely on the first and third exons (exons 1 and 3),respectively. In addition the exon 2 gene comprises the typicalcuticular chitin binding domain (ChBD) type R&R-2 that allowsdirect binding and strong interaction between the resilin andchitin during the process of resilin deposition and constructionof the cuticle composite. Interestingly Ardell and Andersen aswell as the authors of this paper found two splicing resilinmRNA variants CG15920-RA and CG15920-RB which differin the presence of the ChBD (PAKYEFNYQVEDAPSGLSF-GHSEMRDGDFTTGQYNVLLPDGRKQIVEYEADQQGYR-PQIRYEGDANDGSGPSGP).13 Recently Elvin et al. expressedthe first exon (exon 1) of D. melanogaster CG15920 gene in E.coli.11 Cross-linking was used to form a solid biomaterial (Rec1-resilin) via Ru(II)-mediated photo-cross-linking. This materialhad up to 90-92% resilience and could be stretched to over300% of its original length before breaking, based on scanningprobe microscopy and tensile testing.11
In order to understand and assess the functional and structuralproperties of native resilin more completely, we cloned andexpressed the full native resilin protein of the DrosophillaCG15920 gene, which encodes the three exons of the native
* To whom correspondence should be addressed. Tel.: 01-617-627-3251(D.L.K.); 972-8-9489084 (O.S.). Fax: 01-617-627-3231 (D.L.K.); 972-8-9462283 (O.S.). E-mail: email@example.com (D.L.K.); firstname.lastname@example.org (O.S.).
These authors contributed equally to this work. Department of Biomedical Engineering, Tufts University. The Hebrew University of Jerusalem.| Department of Physics and Astronomy, Tufts University.
Biomacromolecules 2009, 10, 32273234 3227
10.1021/bm900735g CCC: $40.75 2009 American Chemical SocietyPublished on Web 11/23/2009
protein (exon 1 + exon 2 + exon 3). The structural and elasticproperties of un-cross-linked and cross-linked full length resilinwere characterized by Fourier transform infrared spectroscopy(FTIR) and atomic force microscopy (AFM). The ChBD R&Rconsensus sequence was identified in 72% of cuticular proteinsthat were discovered from the arthropod kingdom. Neverthelessthere is little experimental evidence showing that these se-quences bind chitin. In this paper we present experimental dataconfirming that the peptide sequence identified as ChBD typeR&R-2 in D. melanogaster resilin confers chitin binding toresilin, implying its role in the formation of the cuticle compositestructure.
Materials and Methods
Gene and Plasmid Construction. Cloning of 6H-res and6H-resChBD Genes. RNA was extracted from Drosophila melanogasterpupa using TRI Reagent (Sigma, St. Louis, MO).14 Reverse transcriptionof the resilin cDNA was performed with M-MLV RT (H-) (Promegacorporation, Madison, WI) with oligo(dT)15 primer according to themanufacturers instructions (Supporting Information, part IV). ThecDNA was used as template for production of 975 and 1200 base pairproducts coding for the first exon elastic repeats (6H-res, amino acids18-324) and with the ChBD (6H-resChBD amino acids 19-415),respectively (Figure 1). Resfor, 5-CCATGGGACCGGAGCCAC-CAGTTAACTC-3, was used as the forward primer for the amplifica-tion of both constructs. Resbmh1_rev, 5-GGATCCCTCATCGT-TATCGTAGTCAGCG-3, was used as the reverse primer foramplification of 6H-res. ResChBDRev, 5-GGATCCTTAAGGAC-CGCTGGGACCACTG-3, was used as the reverse primer for ampli-fication of 6H-resChBD. The genes were amplified using the followingPCR method: 94 C for 4 min, 35 cycles of 94 C for 1 min, 56 C for1 min. 72 C for 1 min, 72 C for 4 min. The genes were cloned usingNcoI and NotI into pHis-parallel-3 vector (http://wolfson.huji.ac.il/expression/local/parallel/pHis-Parallel3.jpg), which contain an N-ter-minal His tag and a rTev cleavage site enabling purification of theprotein on Ni-NTA column and removal of the His tag when desired.
Cloning of Nontagged Full Length Resilin. The full length resilinexpression primers were 1PAF and 3PAR. Their sequences were 1PAF,5-GGAATATGTTCAAGTTACTCGCGTTGACGCTGCTCATGGC-3, and 3PAR, 5-CTAGTACCGATAACCGCTGCCATCGTTGT-CACCGTTCTGA-3. These primers for PCR were designed to amplifythe three exons of the proposed D. melanogaster resilin gene, CG15920.13 Reagents were purchased from Invitrogen (Carlsbad, CA),and the following reaction mixture was used for amplification of allexons of resilin: 5 L Pfx reaction mix (22 U/mL Thermococcus speciesKOD thermostable polymerase complexed with anti-KOD antibodies,66 mM Tris-SO4 (pH 8.4), 30.8 mM (NH4)2SO4, 11 mM KCl, 1.1 mMMgSO4, 330 M dNTPs, AccuPrime proteins, stabilizers), 0.5 L (5U/L) AccuPrime platinum Pfx polymerase, 1 L (20 mM) forwardprimer, 1 L (20 mM) reverse primer, 37.5 L distilled water, and 5L mixture of first strand cDNA synthesis reaction. The followingthermocycler program was used to amplify full length resilin gene:denature at 95 C for 2 min; 35 cycles of 95 C for 15 s, 55 C for15 s, 68 C for 1 min per kb to be amplified; and 68 C for 10 min.The PCR products were analyzed using agarose gel electrophoresis and
purified by gel extraction. The PCR product (1818 bp) was insertedinto the pCR-Blunt II-TOPO vector (Invitrogen Carlsbad, CA) andclones were selected for resistance to ampicillin (100 g/mL). The fulllength resilin DNA fragment was prepared for insertion into the bacterialT7-promoter expression vector pET22b (Novagen EMD Chemicals,Inc. CA) by partial digestion with NcoI and NotI. The NcoI/NotIfragment was inserted between the corresponding sites of pET22b; therecombinant expression plasmid, pET22b/Res, was isolated from E.coli NEB5R cells (NEB, MA) with selection for ampicillin resistance(100 g/mL) and the correct construct was verified by DNA sequenceanalysis. Full details are provided in the Supporting Informationincluding the DNA and amino acid sequence analysis of full lengthresilin.
Expression. All expression vectors were transformed into BL21 Star(DE3; Invitrogen Carlsbad, CA). Authenticity of the clones wasconfirmed by DNA sequencing. A total of 5 mL of overnight cultureswere grown in LB medium with 100 g/mL ampicillin at 37 C in arotary shaker and were used for inoculation of 1 L of LB cultures with100 g/mL ampicillin at a ratio of 1/100 of starter to culture volume.At O.D.600 of 0.8-0.9 expression was induced with 1 mM IPTG.Following 4-6 h from induction, bacteria were harvested by centrifu-gation (10000 g for 20 min at 4 C). Pellets were stored at -80 C.
Purification of Full Length Resilin. The cell pellets were thawedand resuspended in lysis buffer containing 1 BugBuster ProteinExtraction Reagent (Novagen EMD Chemicals, Inc. CA), LysonaseBioprocessing Reagent (Novagen EMD Chemicals, Inc. CA), and 1phosphate-buffered saline. The cell suspension was lysed with shakingfor 1 h. The soluble protein fraction was collected by centrifugation at10000 g for 1 h at 4 C. The resulting supernatant was heated for 30min at 90 C and denatured proteins were removed by centrifugationat 10000 g for 30 min at 20 C. A total of 20% solid ammonium sulfatewas added to remove bacterial proteins, and 30% salt was then used toprecipitate the recombinant resilin. Precipitating proteins were resus-pended in sterile phosphate-buffered saline (PBS), and dialyzedovernight at 4 C in excess PBS. Purity and recovery rates were assessedby SDS-PAGE on 4-12% Bis-Tris precast gels (Invitrogen, CA).
Purification of Recombinant 6H-res and 6H-resChBD. Bacterialpellets recovered from 1 L fermentation broth were resuspended in 75mL of 20 mM Na-phosphate, 0.5 M NaCl, 25 mM imidazole withComplete protease inhibitor (Roche, Switzerland) followed by soni-cation in ice bath. The soluble fraction was separated by centrifugationat 10000 g for 45 min at 4 C. Cleared bacterial lysates were filteredwith a 0.45 M syringe membrane followed by affinity chromatography(AC) on HisTrap HP Ni-NTA pre-equilibrated 5 mL column mountedto AKTAprime plus FPLC (GE, Sweden). The recombinant proteinswere purified as follows: buffer A (binding), 20 mM NaHPO4, 0.5 MNaCl, 10 mM imidazole; buffer B (elution), 20 mM NaHPO4, 0.5 MNaCl, 0.5 M imidazole; (1) 2 column volumes (CV) of buffer A at 5mL/min, (2) 75 mL injection of the lysate at 5 mL/min, (3) 5 CV washwith the buffer A, (4) 5 CV step of 10% buffer B, (5) 7 CV step of100% buffer B, (6) equilibration with 5 CV of binding buffer at 1 mL/min. The eluted proteins were detected at O.D. 280. Approximately400 L fractions were collected and 10 L of samples boiled withSAB were loaded on a 12.5% SDS-PAGE gel. Subsequently, the ACpurified fractions were pooled and diluted with 20 mM Na-phosphatebuffer to EC < 4 mS followed by ion exchange chromatography (IEC)on a 5 mL HiTrap Q FF column as follows: buffer A (binding), 20mM NaHPO4; buffer B (elution), 20 mM NaHPO4, 0.5 M NaCl; (1) 2column volumes (CV) of buffer A at 5 mL/min, (2) injection of thediluted pooled AC fractions at 5 mL/min, (3) 5 CV wash with the bufferA, (4) 5 CV step of 30% buffer B, (5) 8 CV step of 60% buffer B, (6)5 CV of step of 100% buffer B, (7) equilibration with 5 CV of bindingbuffer at 1 mL/min. The purified proteins were analyzed by 12.5%SDS-PAGE and stained with Coomassie blue.
Chitin Binding. Qualitative binding assay was performed both withcrude bacterial lysates and IEC purified proteins using chitin beads(NEB, MA). A total of 50 mg chitin beads were washed once with
Figure 1. Amino acid sequence of 6H-resChBD. Italics mark theN-terminal tail; bold letters mark the ChBD that is missing in 6H-resprotein.
3228 Biomacromolecules, Vol. 10, No. 12, 2009 Qin et al.
PBS followed by addition of 50 g recombinant proteins in 500 LPBS. The mixture was incubated under gentle shaking for 30 min atRT followed by centrifugation. The supernatant was removed (unboundfraction) and the pellets were washed with 500 L of PBS. Precipitatedchitin pellets with bound proteins were boiled with 50 L of 2 sampleapplication buffer (SAB). Unbound and bound proteins were analyzedby SDS-PAGE. For quantitative chitin binding assay, 50 mg of chitinbeads were added to 1.5 mL test tubes and washed once with PBS.Serial dilutions of IEC purified 6H-resChBD (0.4, 1.1, 2.2, 4.3, 8.6,17.2, 21.5 M) were incubated with the chitin beads (three replicatesfor each protein concentration) under gentle shaking for 30 min at roomtemperature. Subsequently, the supernatant was removed (unboundfraction) and the amount of bound proteins was determined using Lowryprotein assay. The maximum amount of bound protein Bmax and Kdvalues were determined by nonlinear regression of the binding isothermsusing a modified model for saturation binding, comprising one bindingsite as developed by Swillens et al.36
The equation B ) (F Bmax)/(Kd + F) used for the calculation,fits nonlinear regression for one binding site, where B is bound proteinand F is free protein. The results were analyzed using GraphPad Prism5 software (GraphPad software Inc., CA).
Cross-Linking of Recombinant Resilin. A total of 5 mg oflyophilized recombinant resilin was dissolved in 100 L of 0.25 Msodium borate/boric acid buffer, pH 8.4, forming a solution of resilinwith concentration of 50 mg/mL. As described by Malencik andAnderson,15 the solution was incubated at 37 C for 1 h, and then 250L of a 1 mg/mL solution of horseradish peroxidase (Sigma, MI) wasadded. Subsequently, 10 mM hydrogen peroxide was added to initiatethe cross-linking reaction. The solution was allowed to incubate at 37C for 1 h. Successful cross-linking was checked by gel electrophoresisand fluorescence detection with a microplate spectrofluorometer (Mo-lecular Devices, CA).
Biomaterial Properties. Conformation. Resilin samples were freeze-dried and the structural characteristics were observed using Fouriertransform infrared spectroscopy (FTIR) as previously reported by Huet al.16,17 The fractions of secondary structural components includingrandom coil, R-helices, -strands, and turns were evaluated usingFourier self-deconvolution (FSD) of the infrared absorbance spectra.FSD of the infrared spectra covering the amide I region (1595-1705cm-1) was performed by Opus 5.0 software. The second derivative wasfirst applied to the original spectra in the amide I region with a nine-point Savitsky-Golay smoothing filter. Deconvolution was performedusing Lorentzian line shape with a half-bandwidth of 25 cm-1 and anoise reduction factor of 0.3.16,17 Circular dichroism (CD) spectra werealso studied for the secondary structure of resilin samples as previouslydescribed.18 All spectra were recorded on an AVIV Model 410spectrophotometer (AVIV Biomedical, Inc., Lakewood, NJ) at roomtemperature (25 C) using a 1 mm path length quartz cell with a 1 nmbandwidth. CD spectra were measured for un-cross-linked and cross-linked full length resilin in the 1 PBS (pH 7.4) with concentrationsin the range of 3.0-5.0 mg/mL. CD data were analyzed using aDICHROWEB program (http://dichroweb.cryst.bbk.ac.uk).19,20
Mechanical Properties. Resilience is defined as the energy recov-ered after removal of the stress divided by the total energy ofdeformation.11,21 The elastic properties of the full length and cross-linked resilins were performed using AFM as previously described.8,11,21
A force-distance curve was obtained for evaluation of materialproperties. Resilin samples were dried on the surface of mica.Measurements on the full length recombinant resilin and cross-linkedresilin were conducted using AFM operated in force mode. A total of10 independent trials were performed for resilin samples and mica wasused as controls to calibrate the instrument. Resilience is given bycalculating the ratio of the areas under the penetration and retractioncurves in the force-distance curves.8,11,21
Gene Construction, Protein Purification, and Cross-Link-ing of Full Length Resilin. PCR amplification was used tosuccessfully prepare the full length gene to construct the plasmidpET22b/Res containing the full length 1818 bp resilin gene(Figure 2A). After the plasmid pET22b/Res was transformedinto E. coli strain BL21 Star (DE3), the expression was carriedout for 6 h at 37 C. Using a heat and salting-out method, theresilin protein was purified (Figure 2B). The final purified yieldwas about 20 mg/L of culture. N-Terminal amino acid sequenceanalysis of the purified resilin revealed the expected amino acidsequence (MVRPEPPVNSYLPPSDSYGA).
Successful formation of cross-linked resilin was obtainedusing horseradish peroxidase. Cross-linked samples showed highmolecular weight which barely entered the 4-12% SDS-PAGEgel, indicating significant polymerization (Figure 2C). Fluoro-metric analysis also indicated cross-links, with absorption andemission maxima at 320 and 400 nm, respectively. Based onthe fluorometric analysis results (Figure 2D), the fluorescenceof this cross-linked resilin was higher than that of full lengthresilin. During the purification, full length resilin exhibited heatstability up to 100 C for 30 min. Generally, heat stability isdependent upon several factors, including time, temperature andantioxidants. Many structural proteins exhibit heat stability. Inour studies, following heating of the culture supernatant at 60,70, 80, 90, and 100 C for 30 min, many proteins are denaturedand precipitated, but the full length resilin proteins remainedintact even after treatment at 100 C for 30 min.
Construction, Expression, and Purification of 6H-resilingenes. Sequencing of cDNAs prepared from D. melanogatserpupas revealed the presence of the two spliced variants asreported previously (Supporting Information, part IV).13 VariantA that contains the ChBD was used for further work. The 975and 1200 base pair products coding for resilin elastic repeatswith or without the ChBD, respectively (6H-resChBD, aminoacids 19-415; 6H-res, amino acids 18-324, Figure 1), wereexpressed in E. coli. 6H-res protein was produced as control toconfirm that the chitin binding is conferred by the putativeChBD. In early experiments we discovered that the chitinbinding ability of resilin was abolished due to the heat treatment(data not shown), therefore, a different purification approachwas used for chitin binding experiments. Both proteins wereexpressed in E. coli and yielded approximately 100 mg/L ofsoluble protein, significantly more than the full length protein.Crude lysates were affinity purified by Ni-NTA chromatography(AC; Figure 3A,B) followed by IEC on Q-Sepharose column(Figure 3C,D). The affinity to chitin was assayed using bothcrude and pure proteins. Specific chitin binding was evidentonly for 6H-resChBD (Figure 4). Equilibrium adsorptionisotherms were conducted and a Kd of 1.6 M and Bmax of 0.082mol/g were calculated from a nonlinear regression of theadsorption isotherms (Figure 5).
Conformational Properties. Conformational properties offull length resilin have not been previously investigated. BothFTIR and CD spectroscopies were employed to probe thesecondary structure of full length resilin before and after cross-linking. The FTIR spectra of un-cross-linked and cross-linkedfull length resilins are shown in Figure 6A,B, which includesan expansion of the amide I region for secondary structureanalysis. The broad nature of the amide I bands (centered around1650 cm-1) indicates a wide range of heterogeneous conforma-tions, and peak deconvolution suggested potential contributionsfrom all known secondary structures (Table 1). The bandbetween 1635 and 1655 cm-1 (centered around 1650 cm-1)
Recombinant Chitin Binding Resilin Biomacromolecules, Vol. 10, No. 12, 2009 3229
exhibited characteristics of random coil configurations (morethan 40%). This high degree of disorder is also consistent withthe observed CD spectra (Figure 6C). Deconvolution of the CDspectrum suggests the minor contributions from coexistingsecondary structures, indicating a largely unordered structure.The cross-linked resilin and the un-cross-linked full length resilinhad similar FTIR and CD spectra, suggesting the similarity inthe conformational properties of both samples (Table 1). Thesedata indicate that the full length recombinant resilin chains aremobile, and sample a wide range of conformations, which isalso the case for the cross-linked resilin.
Mechanical Properties of Full Length and Cross-LinkedResilin. Resilience is a measure of the ability of a material todeform and recover and it has become routine to use AFM tomeasure the modulus or stiffness of materials with resolutionof nanometers, similar to a conventional compression tests.21
Force-distance curves for both samples are shown in Figure7. Compared with 92% resilience of the partial resilin clone,rec1-resilin,11 the full length resilin was 94 ( 1% and 96 (
2% for the cross-linked material. Thus, the full length proteinoffered similar material functions to the partial clone. Thisresilience is superior to that of a known low-resilience rubbers,such as chlorobutyl rubber (56%), and even to high-resiliencepolybutadiene rubbers (80%).11
DiscussionElastic proteins are characterized by being able to undergo
significant deformation, without rupture, before returning to theiroriginal state when the stress is removed. The sequences ofelastic proteins contain repeated sequences of elastomericdomains, and additional domains that form intermolecular cross-links.5 Only a few elastomeric proteins, especially elastin,abductin, and flagelliform spider silks, have been studied formechanical and biochemical properties, and their potential asbiomaterials for industrial and biomedical applications have beendocumented.7,8,22,23 However, other elastic proteins, includingresilin, have not been studied in such detail due to the difficultiesin obtaining large amounts of pure resilin from natural sources.
Figure 2. Gene construction, protein purification and cross-linking of soluble full length resilin. (A) Gene construction: lane 1, pET22b vectordigested by NcoI and NotI; lanes 2-3, pET22b/Res plasmid digested by NcoI and NotI. Expected size of digestion product is 1818 bp (arrow).Size marker is Quick-load 1 kb DNA ladder (New England Biolabs) in lane 4. (B) 4-12% SDS-PAGE of samples from purification: lanes 1-4,cleared supernatant from lysed cells expressed for 0, 2, 4, 6 h; lane 5, precipitation from lysed cells expressed for 6 h; lane 6, soluble full lengthresilin purified by a heat and salting-out method (arrow). Seeblue plus2 prestained standard (Invitrogen, CA) was used as size markers. (C)HRP-cross-linking: The solution containing 50 mg/mL soluble full length resilin, 1 mg/mL HRP, and 10 mM hydrogen peroxide produces polymerizedresilin, which barely enters the gel (arrow); lane 1, mixture with H2O2; lane 2, mixture without H2O2. Seeblue plus2 prestained standard (Invitrogen)was used as size markers. (D) Fluorescence of full length resilin. The absorption and emission maxima were 320 and 400 nm, respectively, forthe full length and cross-linked resilins.
3230 Biomacromolecules, Vol. 10, No. 12, 2009 Qin et al.
Recently, a recombinant resilin-like protein (Rec1) wasexpressed, purified by an immobilized metal affinity chroma-tography (IMAC), and photochemically cross-linked to forman elastic biomaterial (Rec1-resilin) with exceptional resilience.8,11
Furthermore, the secondary structure of a synthetic proresilin(AN16) based upon 16 repeats from Anopheles gambiae(AQTPSSQYGAP), was investigated by Raman and NMRspectroscopy and showed that AN16 is an intrinsically unstruc-tured and dynamic protein with no apparent R-helical or -sheetfeatures.12
Early attempts to produce the full length protein resulted inits expression mainly in the form of inclusion bodies.24 In thepresent study, we cloned and expressed a soluble form of thefull length resilin protein (approximately 60 kDa) containing
all three exons from D. melanogaster. The full length proteinwas purified based on heat and salting-out. Due to the loss offunction of the ChBD in heat treatments we developed Ni-NTAAC followed by IEC methods that do not compromise theactivity of the ChBD and allowed us to characterize binding tochitin. Over 70% of the cuticular proteins extracted from animalsrepresenting the entire arthropod kingdom contain the conservedR&R sequence. These findings indicate an important role ofthe ChBD (PAKYEFNYQVEDAPSGLSFGHSEMRDGD-FTTGQYNVLLPDGRKQIVEYEADQQGYRPQIRYEGDAN-DGSGPSGP) by anchoring the cuticlar proteins to the chitinduring the assembly of the protein-cuticle composite. Moreover,the fact that the R&R sequence is usually found in cuticleextracts is explained by the high degree of cross-linking of the
Figure 3. Purification of 6H-resChBD with AKTAprime plus FPLC. (A) Ni-NTA affinity FPLC chromatogram. (B) SDS-PAGE analysis of imidazoleeluted protein (fractions 130-140 mL) stained with coomassie blue. (C) Ion exchange FPLC chromatogram. (D) SDS-PAGE analysis of the salteluted protein (fractions 45-55 mL) stained with coomassie blue.
Figure 4. Chitin binding of 6H-resChBD. (A) SDS-PAGE analysis of chitin binding of 6H-resChBD crude lysate: T, total; B, 6H-resChBD affinitypurified by chitin beads. Protein eluted by boiling in sample application buffer. UB, unbound fraction; 4B, SDS-PAGE analysis of chitin bindingof pure 6H-res (left) and 6H-resChBD (right); T: total protein post IEC purification; B, bound fraction eluted from chitin beads by boiling withsample application buffer; UB: unbound fraction.
Recombinant Chitin Binding Resilin Biomacromolecules, Vol. 10, No. 12, 2009 3231
other protein segments with the chitin that preclude theirextraction.9,13,25,26 Consequently we suggest that the bindingof the cuticular proteins occurs prior to their cross-linking bydityrosine formation, therefore the ChBD is protected from theoxidizing enzymes.
Furthermore the presence of two splice variants of resilincDNA in D. melanogaster (found both by Ardell and Ander-son13 and by us) can be explained by a requirement for a balancebetween chitin bound and free resilin molecules that assemblethe final polymer composite in the cuticle. Furthermore, thelimited available surface of chitin for binding resilin and othercuticular proteins may explain why these two splice variantsevolved.
To produce high molecular weight cross-linked polymericmaterial, a peroxidase that is present in extracts of resilin fromthe adult desert locust (Schistocerca gregaria) was used togenerate solid cross-linked material.8,25 Physical propertiesincluding structure and elasticity characteristics were measuredfor the recombinant full length resilin and the cross-linkedversion. Typically full length resilin contains 39 tyrosines ofthe 605 amino acids (6.4% composition), and resilin can becross-linked because of the covalent cross-links between tyrosineresidues. The amino acid cross-links were identified as di- andtrityrosine by chemical analysis as previously reported.9 Becauseof these amino acids, resilin fluoresces with a bluish color witha maximum emission at 420 nm under ultraviolet light. Theexcitation maximum varies from 285 to 315 nm as the pH goesfrom acidic to alkaline. A maximum cross-linking near 21%dityrosines was formed in the cross-linked rec1-resilin.11 Bycomparison, about 25% of tyrosines occur as dityrosines innatural locust wing hinge resilin.11,26 The full length resilinreported in this paper was cross-linked by HRP and similarlyfluorescent, with the absorption and emission maxima at 320and 400 nm, respectively.
Ardell and Andersen suggested that the amino acid composi-tion of D. melanogaster resilin may induce the formation of-turns that result in a -spiral, which is composed of severalrepetitive -turns which act as spacers between the turns of thespiral, suspending chain segments in a conformational freestate.13 We investigated the secondary structure distribution inthe full length recombinant resilin from D. melanogaster. Themajority of the full length resilin backbone exhibited randomcoil configurations, indicating that the overall protein wasdynamic and unstructured. This high degree of disorder wasalso consistent with the observed CD spectra. For cross-linkedfull length resilin, the structure characteristics were similar tothe un-cross-linked version, which implied that a wide range
of conformations were also present within the cross-linkedproteins. No evidence was found for a -spiral structure inresilin, and these results are consistent with the random-networkelastomer model and the sliding -turn model.27-31 The
Figure 5. Nonlinear regression of 6H-resChBD binding to chitin.Different protein concentrations were incubated with 50 mg chitinbeads as described in materials and methods. Kd (1.62 M) and Bmax(0.082 mol/g) values were calculated from the nonlinear regressioncurve (R 2 ) 0.9232).
Figure 6. Secondary structure analysis of full length and cross-linkedresilins. (A, B) Selected FTIR absorbance spectra of resilin film (A)and cross-linked resilin film (B) in the amide I regions deduced afterFourier self-deconvolution. The heavy line represents the deducedabsorbance band. The light lines represent the contributions to theamide I band. (C) Far-UV CD spectra. All spectra were recorded atroom temperature (25 C) using a 1 mm path length quartz cell withresilin concentrations in the range of 1.0-3.0 mg/mL.
Table 1. Secondary Structure Analysis of Full Length andCross-Linked Resilins by FTIR and CD
full length resilin FTIR 11.9 15.3 29.1 43.8CD 9.8 16.1 17.5 41.6
cross-linked resilin FTIR 14.2 19.9 24.4 41.4CD 9.3 15.7 17.9 42.7
3232 Biomacromolecules, Vol. 10, No. 12, 2009 Qin et al.
similarities in the contribution of disorder conformations in theun-cross-linked and cross-linked full length resilin suggest thatcross-linked resilin retains sufficient chain mobility for elasto-meric behavior (resilience), an important feature for somebiomaterials applications.32-34
Resilience is defined as the energy recovered after removalof the stress divided by the total energy of deformation. Theenergy of deformation/recovery is given by converting force-displacement curves into force-penetration/retraction curves andcalculating the ratio of the areas under the penetration andretraction curves.11,21,31,32 Compared with the 92% resilienceof rec1-resilin,11 the full length recombinant resilin was 94%resilient, compared to 96% for the cross-linked resilin. Thesedata suggest that both the full length and cross-linked resilinshad high rubber efficiency (resilience).
In Nature, resilin must last the entire lifetime of the animal,extending and retracting millions of times. The unique elasticproperties and the abundance of resilin in the jumping organsof arthropods such as froghopper and cat fleas led manyresearchers to the conclusion that resilin is the major constituentin the jumping mechanism of insects.33 This assumption wasrecently brought to doubt by Burrows et al., that showed thatresilin by it self-is not sufficient to store so much energy andmust act as constituent of a composite with the chitin for thepurpose of jumping.29 In the example given by Burrows et al.,the jumping organ of the froghopper insect Aphrophora thepleural arch, is a composite structure containing approximately80% chitinous cuticle and 20% resilin.29
The high elasticity of resilin combined with the strength ofthe chitin in a composite manner enables insects to rapidlyrestore body shape as well as most of the energy required forthe next mechanical movement either flying or jumping. Ourexperiments demonstrate for the first time that the putativeChBD confers specific anchoring of resilin to chitin.
The research findings provide several opportunities for futurestudies. Additional experiments are needed on the resilin solidmaterial to gain further in sight into the properties and potentialapplications for this elastomeric protein. Recently, the recom-binant production of modular polypeptide materials based onthe highly resilient protein resilin was reproted and the proteinsexhibited useful mechanical and cell adhesion behavior.34 Inparticular, clarification of similarities and differences betweenresilin and elastin would be useful, in order to place each in asuitable context, such as for biomaterial-related applications.Composites of resilin and chitin may exhibit more resilientmechanical properties and may be suitable as a tissue engineer-ing scaffolds. For example, composites of solubilized elastinwith collagen and fibrin have been used as a scaffold for tissuerepair of blood vessels.33,35 Similarly, elastin-silk copolymershave been studied for a range of biomaterial applications overthe past decade.36-38 The stability and biocompatibility of resilinin vivo have yet to be reported. However, use of resilin as ascaffold may be of particular interest for the engineering tissues,which need to be subjected to elastic movements for properdifferentiation, such as the pulsating movements of vasculartissues or skin.39 In addition, the data demonstrate that theputative ChBD domain (PAKYEFNYQVEDAPSGLSFGH-SEMRDGDFTTGQYNVLLPDGRKQIVEYEADQQGYRPQ-IRYEGDANDGSGPSGP) confers specific anchoring of resilinto chitin. This insight may be useful to introduce a ChBD-tagwith recombinant resilin-like proteins to improve purificationfrom crude lysates.
Full length recombinant resilin was generated and character-ized. The material features of this protein were compared toprevious studies where partial clones and proteins were gener-ated and found to be comparable in both structure and function.Moreover, we showed that the chitin binding domain has highaffinity to chitin implying for its role in the formation of theresilin-chitin composite in the cuticle.
Acknowledgment. We would like to acknowledge theassistance of Qiang Lu with the AFM. We are also grateful toDr. Hanna Dams-Kozlowska for technical assistance. Supportfrom the NIH P41 Tissue Engineering Resource Center (NIBIB)is gratefully acknowledged.
Supporting Information Available. DNA sequence used forexpression of full length resilin; amino acid sequence of fulllength resilin; DNA sequence analysis of full length resilin:identification of repeat motifs; RT-PCR results of resilin genefrom D. melonogaster. This material is available free of chargevia the Internet at http://pubs.acs.org.
References and Notes(1) Weis-Fogh, T. J. Exp. Biol. 1960, 37, 887907.(2) Bennet-Clark, H. C.; Lucey, E. C. A. J. Exp. Biol. 1967, 47, 5967.(3) Young, D.; Bennet-Clark, H. C. J. Exp. Biol. 1995, 198, 1001
1020.(4) Weis-Fogh, T. J. Mol. Biol. 1961, 3, 520531.(5) Tatham, A. S.; Shewry, P. R. Philos. Trans. R. Soc., B 2002, 357,
229234.(6) Weis-Fogh, T. J. Mol. Biol. 1961, 3, 648667.(7) Gosline, J.; Lillie, M.; Carrington, E.; Guerette, P.; Ortlepp, C.; Savage,
K. Philos. Trans. R. Soc., B 2002, 357, 121132.(8) Lyons, R. L.; Lesieur, E.; Kim, M.; Wong, D. C. C.; Huson, M. G.;
Nairn, K. M.; Brownlee, A. G.; Pearson, R. D.; Elvin, C. M. ProteinEng., Des. Sel. 2007, 20, 2532.
(9) Andersen, S. O. Biochim. Biophys. Acta 1964, 93, 213215.
Figure 7. Elasticity of resilins by AFM. Force-distance curves wererecorded for the full length resilin (A) and cross-linked resilin (B).
Recombinant Chitin Binding Resilin Biomacromolecules, Vol. 10, No. 12, 2009 3233
(10) Elliott, G. F.; Huxley, A. F.; Weis-Fogh, T. J. Mol. Biol. 1965, 13,791795.
(11) Elvin, C. M.; Carr, A. G.; Huson, M. G.; Maxwell, J. M.; Pearson,R. D.; Vuocolo, T.; Liyou, N. E.; Wong, D. C. C.; Merritt, D. J.;Dixon, N. E. Nature 2005, 437, 9991002.
(12) Nairn, K. M.; Lyons, R. E.; Mulder, R. J.; Mudie, S. T.; Cookson,D. J.; Lesieur, E.; Kim, M.; Lau, D.; Scholes, F. H.; Elvin, C. M.Biophys. J. 2008, 95, 33583365.
(13) Ardell, D. H.; Andersen, S. O. Insect Biochem. Mol. Biol. 2001, 31,965970.
(14) Chomczynski, P.; Sacchi, N. Anal. Biochem. 1987, 162, 156159.(15) Malencik, D. A.; Anderson, S. R. Biochemistry 1996, 35, 4375-
4386.(16) Hu, X.; Kaplan, D.; Cebe, P. Macromolecules 2006, 39, 6161-
6170.(17) Hu, X.; Kaplan, D.; Cebe, P. Macromolecules 2008, 41, 39393948.(18) Greenfield, N. J. Nat. Protoc. 2006, 1, 28762890.(19) Whitmore, L.; Wallace, B. A. Nucleic Acids Res. 2004, 32, W668
W673.(20) Whitmore, L.; Wallace, B. A. Biopolymers 2008, 89, 392400.(21) Huson, M. G.; Maxwell, J. M. Polym. Test. 2006, 25, 211.(22) Yoda, R. J. Biomater. Sci., Polym. Ed. 1998, 9, 561626.(23) Martino, M.; Perri, T.; Tamburro, A. M. Macromol. Biosci 2002, 2,
319328.(24) Kim, M.; Elvin, C.; Brownlee, A.; Lyons, R. Protein Expr. Purif. 2007,
52, 230236.(25) Coles, G. S. J. Insect Physiol. 1966, 12, 679691.
(26) Andersen, S. O. Acta Physiol. Scand. Suppl. 1966, 263, 181.(27) Aaron, B. B.; Gosline, J. M. Biopolymers 1981, 20, 12471260.(28) Tamburro, A. M.; Guantieri, V.; Pandolfo, L.; Scopa, A. Biopolymers
1990, 29, 855870.(29) Burrows, M.; Shaw, S. R.; Sutton, G. P. BMC Biol. 2008, 30, 41.(30) Gross, A. J.; Sizer, I. W. J. Biol. Chem. 1959, 234, 16111614.(31) Haas, F.; Gorb, S.; Blickhan, R. Proc. Biol. Sci. 2000, 267, 1375
1381.(32) Karouzou, M. V.; Spyropoulos, Y.; Iconomidou, V. A.; Cornman,
R. S.; Hamodrakas, S. J.; Willis, J. H. Insect Biochem. Mol. Biol. 2007,37, 754760.
(33) Lombardi, E. C.; Kaplan, D. L. Mater. Res. Soc. Symp. Proc. 1993,292, 37.
(34) Charati, M. B.; Ifkovits, J. L.; Burdick, J. A.; Linhardt, J. G.; Kiick,K. L. Soft Matter 2009, DOI: 10.1039/b910980c.
(35) Lefebvre, F.; Droullet, F.; Savin de Larclasuse, A. M.; Aprahamian,M.; Midy, D.; Bordenave, L.; Rabaud, M. J. Biomed. Mater. Res. 1989,23, 14231432.
(36) Megeed, Z.; Cappello, J.; Ghandehari, H. AdV. Drug DeliVery ReV.2002, 18, 10751091.
(37) Swillens, S. Mol. Pharmacol. 1995, 47, 11971203.(38) Capello, J.; Crissman, J.; Dorman, M.; Mikolajczak, M.; Textor, G.;
Marquet, M.; Ferrari, F. Biotechnol. Prog. 1990, 6, 198202.(39) Alper, J. Science 2002, 297, 329330.
3234 Biomacromolecules, Vol. 10, No. 12, 2009 Qin et al.